Radiation Physics and Chemistry 104 (2014) 292–296 Contents lists available at ScienceDirect Radiation Physics and Chemistry journal homepage: www.elsevier.com/locate/radphyschem TL emission spectra measurements using a spectrometer coupled to the Risoe TL/OSL reader Maíra T. Yoshizumi n, Linda V.E. Caldas Instituto de Pesquisas Energéticas e Nucleares, Comissão Nacional de Energia Nuclear (IPEN-CNEN/SP), Av. Prof. Lineu Prestes, 2242, 05508-000 São Paulo, SP, Brazil H I G H L I G H T S A spectrometer based on a CCD detector was coupled to a TL/OSL reader via optical ﬁber. TL emission spectra of well-known TL materials were measured. The measured spectra showed the expected shapes; thus the system proved a good performance. The set-up is very easy to use and it shows good potential to study new materials. art ic l e i nf o a b s t r a c t Article history: Received 6 June 2013 Accepted 6 April 2014 Available online 15 April 2014 A high sensitivity spectrometer (Ocean Optics QE65 Pro) was coupled to the Risoe TL/OSL reader to measure TL emission spectra of four different dosimeters. This spectrometer is based on a Hamamatsu FFT-CCD detector with a 2-D arrangement of pixels (1044 64), which detects luminescence in a range of 200–950 nm. An optical ﬁber was used to guide the signal from the sample to the spectrometer. TL spectra from LiF, CaSO4:Dy, BeO and Al2O3:C detectors were obtained and they are presented in this work. The proposed detection system showed good response; spectra shape, in accordance with the literature, were obtained, validating the system. & 2014 Elsevier Ltd. All rights reserved. Keywords: Thermoluminescence Emission spectrum TL materials 1. Introduction Thermoluminescence is the light emission when certain materials are heated. This phenomenon occurs during the relaxation process in which trapped electrons in crystal defects are released by heating and recombine with holes emitting a photon. Ionizing radiation creates electron–hole pairs that can be quantiﬁed through the thermoluminescence signal. Although the use of thermoluminescence phenomenon for radiation dosimetry ages from the early 1950s (Daniels et al., 1953), the search for new dosimetric materials and for the comprehension of the thermoluminescence mechanism remains nowadays. Thermoluminescent dosimeters are organic or inorganic crystals with defects or imperfections in their crystalline lattices. According to the energy band theory of solids, the crystal defects or imperfections give rise to energy levels localized at the forbidden gap which may trap electrons or holes created by ionizing radiation n Corresponding author. Tel./fax: þ 55 11 31339715. E-mail addresses: [email protected] (M.T. Yoshizumi), [email protected] (L.V.E. Caldas). http://dx.doi.org/10.1016/j.radphyschem.2014.04.014 0969-806X/& 2014 Elsevier Ltd. All rights reserved. incidence. When trapped electrons or holes are stimulated, they may escape to the conduction band and then recombine, emitting luminescence. The luminescent emission wavelength depends on the recombination centre depth. The deeper the recombination centre, the smaller the luminescence wavelength. The emission spectrum of luminescent materials, along with other studies, helps understanding the defects or imperfections in the crystal lattice and the kinematic phenomenon. This is especially interesting when new materials, natural or synthetic, are being studied. The emission spectrum can be measured using monochromators or a set of narrow-band ﬁlters to discriminate the signal wavelength (Fairchild et al., 1978). These conﬁgurations have the advantage of using a photomultiplier tube to collect and amplify the signal, but they have the disadvantage of time-consumption, because only one wavelength is measured at a time. Nowadays, the whole spectrum can be measured at once and with good sensitivity with the new generation of spectrometers (Bakas, 1984). These detectors have a charge-coupled device (CCD) array and can be sensitive from ultraviolet (UV) to near infrared (NIR) region, depending on their conﬁguration. M.T. Yoshizumi, L.V.E. Caldas / Radiation Physics and Chemistry 104 (2014) 292–296 In this work, a spectrometer connected to a Risoe TL/OSL reader via an optical ﬁber was used to perform TL emission spectra measurements. Well-known luminescent materials, like LiF, CaSO4:Dy, BeO and Al2O3:C, were used to test the spectrometric arrangement. 2. Materials and methods The TL emission spectra were measured using a high-sensitivity spectrometer coupled via optical ﬁber to a TL/OSL reader. 2.1. Samples Four different sample pellets were used in this work. All irradiations were carried out using a Gammacell irradiator, Atomic Energy of Canada, with 98.8 TBq activity and 1.18 kGy h 1 dose rate from the Center for Radiation Technology of IPEN. The LiF pellets, with 3.2 3.2 0.9 mm3 dimensions, were annealed at 400 1C for 1 h before irradiation. 80 1C for 24 h treatment was not undertaken, because it was not intended to reduce the intensity of the low temperature peaks (Fairchild et al., 1978). CaSO4:Dy sintered pellets were provided by a national company MRA Industria de Equipamentos Eletrônicos Ltda. The pellets were 6 mm in diameter and 0.8 mm thick disks, and they were annealed at 300 1C for 3 h. BeO pellets were obtained from the laboratory stock. They were 4 mm diameter disks with 0.8 mm thickness. These samples were annealed at 750 1C for 15 min. Al2O3:C disks were obtained by Rexon Inc. They were 5 mm in diameter and with thickness varying from 0.8 to 1.0 mm. According to the manufacturer, the proper annealing treatment is 800 1C for 15 min. 2.2. Stimulation and detection system The stimulated luminescence was measured using a ﬁber coupled spectrometer attached to the Risoe TL/OSL reader, model DA-20 (Fig. 1). A TL/OSL reader, model DA-20, Risoe DTU, Denmark, was used. This reader is equipped with a heating system that uses alternating current controlled by a non-switching continuous full sine wave generator operating at 20 kHz. Samples can be heated up to 700 1C with heating rates from 0.1 to 10 K/s. For the luminescence detection a bialkali photomultiplier tube (PMT), model 9235, PRF Technologies was used. The Risoe reader is also equipped with a 90Sr/90Y beta source. The optical ﬁber used is a customized UV–vis solarizationresistant ﬁber, with 1.0 mm core diameter. This ﬁber presents a relative transmission better than 80% in the range of 250–900 nm Fig. 1. Risoe TL/OSL reader, spectrometer and optical ﬁber used to measure the TL spectra of different samples. 293 and an acceptance angle in air of 251. Bos et al. (2002) calculated that, for samples of 3 mm diameter, a distance up to 10 mm from the sample to the ﬁber entrance the light collection keeps constant. For 5 mm diameter samples this distance is 13 mm. In the case of the Risoe TL/OSL reader, model DA-20, the distance is shorter than 5 mm and it is mostly due to a quartz window used to isolate the sample ambience. Spectra measurements were carried out using a scientiﬁc-grade spectrometer Ocean Optics, QE65 Pro, with a Hamamatsu FFT-CCD detector with a 2-D arrangement of pixels (1044 64). This detector is conﬁgured with a special diffracting grade HC-1 (groove density of 300 mm 1 and spectral range of 750 nm) and a 200 μm entrance slit, which, according to the manufacturer, provides a pixel resolution of 8.9 pixels. The sensitive wavelength region is from 200 to 950 nm and the wavelength resolution is 6.5 nm FWHM. The detector is totally plug-and-play type, and the software is provided with it. Data unique to each detector is recorded into a memory chip and can be easily accessed through software. Measurements from 8 ms to 15 min can be performed due to its low dark count, high stability and integrated cooling system. The manufacturer previously calibrated the spectrometer on wavelength. This calibration may be repeated after a period of time, but as the equipment is brand-new, this calibration was not performed yet. A relative calibration of the system efﬁciency was obtained using a tungsten–halogen light source. This means that all measurements are relative to that of a blackbody light source with known color temperature. 3. Results and discussion Using the equipment showed in Fig. 1, the TL spectrum of different luminescent materials was measured. These materials were previously irradiated, and the reading parameters were the same for all samples. The absorbed dose used was very high, not applicable to personal dosimetry, but it was necessary to obtain a deﬁned signal and to observe luminescence from different recombination centers. Fig. 2 shows the TL spectrum of a LiF pellet irradiated to 100 Gy (60Co). The luminescence was integrated over 3 s with a heating rate of 2 1C/s. This sample shows a broad dosimetric peak centered around 410 nm. There are many articles about the LiF luminescence response. Although the spectrometric system measured the LiF luminescence showing the dosimetric peak, some details of its emission cannot be noticed. Another measurement with a higher dose was also taken. In Fig. 3, it is possible to see a high deﬁnition LiF TL spectrum. For this measurement the sample was irradiated to 1 kGy (60Co), and it was heated at a rate of 5 1C/s. From Fig. 3 it is also possible to observe minor emissions at longer wavelengths which cause the appearance of a shoulder, but it is not possible to resolve these peaks. The four glow peaks (peak 2 to peak 5) can easily be observed besides the complex peaks at higher temperatures. Results are consistent with the literature (Piters et al., 1993). In Fig. 4, a CaSO4:Dy emission spectrum is shown. The sample was irradiated to a dose of 100 Gy (60Co), and its luminescence was integrated for 2 s during a heating rate of 2 1C/s. The main dosimetric peak around 270 1C is composed mostly by two dominant emission bands at 480 and 580 nm as expected (Piters et al., 1993). The sharp lines seen in Fig. 4d are characteristic of the rare earth dopant (Dy). The CaSO4:Dy glow curve and the mechanisms of the defect structure are very complex, but this material showed the best TL sensitivity among the studied materials. The BeO sample presents only one broad peak; however, this peak apparently consists of an overlapping of other components 294 M.T. Yoshizumi, L.V.E. Caldas / Radiation Physics and Chemistry 104 (2014) 292–296 Fig. 2. (a) Isometric plot of TL spectrum of LiF (100 Gy; Fig. 3. (a) Isometric plot of TL spectrum of LiF (1 kGy; 60 60 Co) heated at 2 1C/s, (b) contour plot and (c) and (d) spectrum proﬁles. Co) heated at 5 1C/s, (b) contour plot and (c) and (d) spectrum proﬁles. M.T. Yoshizumi, L.V.E. Caldas / Radiation Physics and Chemistry 104 (2014) 292–296 Fig. 4. (a) Isometric plot of TL spectrum of CaSO4:Dy (100 Gy; Fig. 5. (a) Isometric plot of TL spectrum of BeO (100 Gy; 60 60 Co) heated at 2 1C/s, (b) contour plot and (c) and (d) spectrum proﬁles. Co) heated at 2 1C/s, (b) contour plot and (c) and (d) spectrum proﬁles. 295 296 M.T. Yoshizumi, L.V.E. Caldas / Radiation Physics and Chemistry 104 (2014) 292–296 Fig. 6. (a) Isometric plot of TL spectrum of Al2O3:C (100 Gy; 60 Co) heated at 2 1C/s, (b) contour plot and (c) and (d) spectrum proﬁles. (Fig. 5). It is centered at 330 nm, and it shows a shoulder to longer wavelengths. The glow curve of BeO depends upon the origin of the material, and the peak shifts with the absorbed dose (McKeever et al., 1995). The TL emission spectrum of Al2O3:C is shown in Fig. 6. The sample was irradiated to a dose of 100 Gy (60Co), and its luminescence was integrated for 2 s during a heating rate of 2 1C/s. The expected glow curve for Al2O3:C is a single peak centered at approximately 210 1C (at a heating rate of 10 1C/s), but this material presents strong thermal quenching, and the peak shifts to higher temperatures due to increasing heating rates. The maximum emission peak, at 410 nm, is caused by electrons trapped on F þ centers (Summers, 1984). 4. Conclusions Well-known TL materials were used to test a spectrometric system, which is based on a CCD detector coupled directly to a TL reader via optical ﬁber. The TL spectrum of these materials was obtained, and it was possible to observe the expected characteristics of each spectrum. LiF pellets present four glow peaks, so a higher dose (1 kGy) was necessary to see these peaks. CaSO4:Dy, BeO and Al2O3:C present a single glow peak, which consist of an overlapping of other components, and a dose of 100 Gy was enough to obtain a good response. The heating rate was kept very low compared to that of routine, 2 1C/s, because at low rates the luminescence process is optimized. This system showed good potential to study new materials, once it is very easy to use, and it showed a good performance. Acknowledgments The authors thank the Brazilian agencies FAPESP (Grant no. 2011/20935-9), CNPq, CAPES and MCTI (INCT—Radiation Metrology in Medicine project), for partial ﬁnancial support. References Bakas, G.V., 1984. A new optical multichannel analyser using a charge coupled device as detector for thermoluminescence emission measurements. Radiat. Prot. Dosim. 9, 301–305. Bos, A.J.J., Winkelman, A.J.M., Le Masson, N.J.M., Sidorenko, A.V., van Ejik, C.W.E., 2002. A TL/OSL emission spectrometer extension of the Risoe reader. Radiat. Prot. Dosim. 101, 111–114. Daniels, F., Boyd, C.A., Saunders, D.F., 1953. Thermoluminescence as a research tool. Science 117, 343–349. Fairchild, R.G., Mattern, P.L., Lengweiler, K., Levy, P.W., 1978. Thermoluminescence of LiF TLD-100: emission spectra measurements. J. Appl. Phys. 49, 4512–4522. McKeever, S.W.S., Moscovitch, M., Townsend, P.D., 1995. Thermoluminescence Dosimetry Materials: Properties and Uses. Nuclear Technology Publishing, England. Piters, T.M., Meulemans, W.H., Bos, A.J.J., 1993. An automated research facility for measuring thermoluminescence emission spectra using an optical multichannel analyzer. Rev. Sci. Instrum. 64, 109–117. Summers, G.P., 1984. Thermoluminescence in single crystal α-Al2O3. Radiat. Prot. Dosim. 8, 69–80.